Influence of HALO and drain-extension doping gradients on transistor performance
Page content transcription
If your browser does not render page correctly, please read the page content below
Materials Science and Engineering B 114–115 (2004) 15–19 Influence of HALO and drain-extension doping gradients on transistor performance Axel Erlebacha,∗ , Thomas Feudelb , Andreas Schenkc , Christoph Zechnera a ISE AG, Affolternstr. 52, 8050 Zurich, Switzerland b AMD Saxony LLC and Co. KG, Wilschdorfer Landstrasse 101, D-01109 Dresden, Germany c ETH Zurich, Integrated Systems Laboratory, Gloriastr. 35, CH-8092 Zurich, Switzerland Abstract For achieving a physical gate length lower than 50 nm and keeping at the same time good transistor performance, a careful design of drain-extension and channel doping profiles is required. For this we investigate the influence of drain-extension and HALO doping gradients at the drain-extension channel junction (DECJ). It is found that the influence of the drain extension doping gradient on the threshold voltage roll-off behavior is small for steep profiles when keeping saturation current and overlap capacitance constant. On the other hand, the shape of the HALO profile influences the threshold voltage roll-off characteristics and allows to adjust the roll-off behavior without degrading the saturation current dramatically. The effect of process parameters like HALO implantation angle and energy on the transistor performance is studied. © 2004 Published by Elsevier B.V. Keywords: Drain-extension; Doping; Transistor; HALO; Threshold voltage roll-off; Saturation current 1. Introduction order to have high Ion . Concluding, one has to find a trade- off between improving the threshold voltage roll-off behavior For very deep sub-m technologies, down scaling and and keeping constant Ion and overlap capacitance Cov . transistor performance are strongly connected with the design A simple increase of channel doping concentration would of appropriate doping profiles close to the drain-extension give a higher stability against gate length variations and a low channel junction (DECJ) under the gate. Thereby, the roll- Ioff value. However, this way one also has to accept a higher off behavior of the threshold voltage as well as the saturation threshold voltage and a lower mobility in the inversion layer current play an important role and are in the focus of attention and, as a consequence, a lower saturation current. The im- in improving transistor performance. The goal is to get a high provement of the roll-off behavior can also be achieved by stability of threshold voltage against gate length variation increasing the doping profile gradient of the drain-extension for gate lengths close to the value of the nominal transistor, profile. The price one has to pay is an increase of the thresh- to obtain high saturation current Ion (Ion : drain current at old voltage and a degradation of the saturation current for the Vg = Vdd and Vd = Vdd , Vdd : operating voltage), and low nominal gate length. Optimizing HALO implantation dose Ioff current (Ioff : drain current at Vg = 0 V and Vd = Vdd ) and distance between DECJ and gate edge in order to com- simultaneously. On the one hand, this means to suppress both pensate for the change of threshold voltage, saturation cur- the punch through from the drain side and the lowering of rent, and overlap capacitance, results in a worsening of the the source-channel potential barrier. On the other hand, one roll-off behavior. Therefore, one needs to find another way needs to decrease the source-channel potential barrier and in order to improve the threshold voltage roll-off behavior. thus, the net concentration at the channel side of the DECJ in The main tools used for the present investigation are 2D process and device simulation with DIOSISE  for process ∗ Corresponding author. and DESSISISE  for device simulation, respectively. The E-mail address: email@example.com (A. Erlebach). process simulator is applied to generate doping profiles and 0921-5107/$ – see front matter © 2004 Published by Elsevier B.V. doi:10.1016/j.mseb.2004.07.022
16 A. Erlebach et al. / Materials Science and Engineering B 114–115 (2004) 15–19 device structures. The simulated drain-extension and chan- Table 1 nel profiles are adjusted to match typical device data of very Saturation current for different drain-extension doping gradients with and without compensation of saturation current degradation and overlap capac- deep sub-m technologies like threshold voltage, saturation itance lowering current, junction depth, and overlap capacitance. However, Variant Ion (A) no specific calibration is done and many process steps are simplified. Device simulation is performed with the drift dif- A 590 B 360 fusion model using quantum corrections. The parameter set C 490 of Darwish  is used for the inversion layer mobility. The D 530 poly depletion effect is taken into account by solving the E 550 Poisson equation in the poly silicon gate. It is well-known (A: offset = 4 nm/low doping gradient, B: offset = 1 nm/high doping gradient, that quasi-ballistic effects play an important role in the case C: offset = 1 nm/high doping gradient, D: offset = 1 nm/high doping gradient, of ultra-short gates. Monte Carlo device simulation [4,5] is E: offset = 1 nm/high doping gradient). The HALO dose for the variants A, B, and C is 4.0 × 1013 cm−2 , whereas the HALO dose for the variants D therefore, well suited for those investigations, whereas hy- and E is 3.5 × 1013 cm−2 and 3.0 × 1013 cm−2 respectively. The saturation drodynamic and drift diffusion models give either too high current is always for a constant Ioff of 10 nA. or too low values for the saturation current. However, since Monte Carlo simulation still requires too much computation 2. Inﬂuence of drain-extension proﬁle on threshold time, it can hardly be used for daily industrial applications voltage roll-off behavior where many different process and device variants have to be considered. Thus, we fit the high-field mobility in the drift Fig. 1 presents the influence of the drain-extension dop- diffusion model to MC simulation results and then perform ing gradient on the threshold voltage at a drain bias of 1 V. all other simulations with the calibrated drift diffusion model. The threshold voltage is determined at a drain current level of The resulting failure will most probably not change the influ- 0.1 A, where the current is normalized by the gate length. ence of the doping concentration on the electrical transistor The slope of the drain-extension profile is varied between 2 behavior. and 10 nm per decade, where an abruptness of 3. . .5 nm per In chapter II, we show results of the investigation of the in- decade is required for a gate length of 32. . .37 nm according fluence of the drain-extension doping gradient on the thresh- to the ITRS roadmap . Fig. 1 clearly shows that steeper old voltage roll-off characteristics. Chapter III explains the profiles result in a better roll-off behavior. On the other hand, effect of the compensation of threshold voltage shift and satu- the threshold voltage is strongly increased by about 100 mV ration current degradation by the adjusting distance between for the longest channel considered here. The increase of the DECJ and gate edge and by decreasing the HALO implanta- threshold voltage causes a decrease of the saturation current tion dose. The last section, investigates the influence of the due to the lowering of the inversion charge. The saturation shape of the HALO profile on the roll-off curves. current is further degraded by the lowering of the mobility Fig. 1. Dependency of threshold voltage on gate length for different drain-extension doping gradients with and without compensation of saturation current and overlap capacitance lowering (A: offset = 4 nm/low doping gradient, B: offset = 1 nm/high doping gradient, C: offset = 1 nm/high doping gradient, D: offset = 1 nm/high doping gradient, E: offset = 1 nm/high doping gradient). The HALO dose for the variants A, B, and C is 4.0 × 1013 cm−2 , whereas the HALO dose for the variants D and E is 3.5 × 1013 cm−2 and 3.0 × 1013 cm−2 , respectively.
A. Erlebach et al. / Materials Science and Engineering B 114–115 (2004) 15–19 17 due to the higher doping concentration (higher doping con- centration results in higher electric field at the silicon-oxide interface). The higher threshold voltage is always connected with a lower Ioff , whereas the mobility degradation affects mainly the saturation current. The overlap capacitance is re- duced by about 50%. For a fair evaluation of the different variants (see Table 1), we have to compare the saturation cur- rents at constant Ioff . For each variant the same Ioff of 10 nA is adjusted and the saturation current is extracted. In Table 1 we see that the saturation current of variant B drops down by a factor of two compared to all other variants. Therefore, the in- crease of the abruptness of the drain-extension profiles results in a strong degradation of the saturation current. The differ- ent compensation methods reduce the degradation. However, Fig. 2. Explanation of the influence of the doping gradient on channel length and net doping concentration. they also cancel out the improvement of the threshold voltage roll-off behavior. threshold voltage. The goal is therefore to re-adjust the sat- uration current by lowering the HALO implantation dose. Because this is accompanied by a decrease of the doping con- 3. Compensation of degradation of saturation centration at the DECJ, the space charge region towards the current channel at the source and drain sides will be enlarged. This again makes the roll-off behavior worse, partially canceling The increase of the abruptness of the drain-extension pro- the improvement achieved by increasing the drain-extension file results in a degradation of the saturation current. This is doping gradient (see Fig. 2). a collateral effect of the improvement of the roll-off behavior The main problem of the compensation methods discussed and has to be corrected in order to obtain the same perfor- above is the degradation of the improvement of the threshold mance of the nominal transistor as before. The correction can voltage roll-off behavior achieved by increasing the drain- be done by tuning the offset between gate edge and DECJ and extension doping gradient. The degradation of the saturation by decreasing the HALO dose. current is compensated by lowering the HALO dose from 4.0E13 to 3.0E13 cm−2 and by increasing the overlap be- 3.1. Distance between DECJ and gate edge tween drain-extension and gate by 3 nm. As one can clearly see, the compensation completely cancels the improvement The change of the drain-extension doping gradient results of the threshold voltage roll-off behavior. in a change of the overlap capacitance, where steeper profiles give less capacitance. For some configurations and very steep profiles one can even obtain a degraded transistor without any 4. Inﬂuence of shape of the HALO doping proﬁle on overlap resulting in a high channel resistance and a very low transistor performance saturation current. In order to keep the overlap capacitance constant the distance between DECJ and gate edge is varied After the necessary adjustments for avoiding the degra- using selected process parameters. This mainly results in a dation of the saturation current, the possibilities to use the lateral shift of the drain-extension profile and, therefore, in drain-extension doping gradient for improvements of the roll- a change of the effective channel length. When increasing off behavior are limited. However, the shape of the HALO the doping gradient of the drain-extension profile one has to profile close to the DECJ gives another opportunity to im- generate a shift of the junction of 2–5 nm on both sides of the prove the roll-off behavior without degrading the saturation channel in order to correct for overlap capacitance and sat- current too much. In this case the goal is to minimize the size uration current. This correction cancels already a part of the of the space charge region at the lateral junction and to raise improvement of the roll-off curve. Fig. 2 explains the effect of increasing the drain-extension doping gradient and of com- Table 2 pensating the current degradation and overlap capacitance Saturation current for different HALO implantation energies with Ioff kept lowering by shifting the DECJ back to the former position. constant at 10 nA HALO implantation energy (keV) Ion (A) 3.2. HALO implantation dose 2 380 4 485 The doping gradient of the extension profile changes also 6 510 the doping concentration at the channel side of the DECJ. 8 555 A higher drain-extension doping gradient is connected with 10 560 12 580 a higher channel doping concentration. This increases the
18 A. Erlebach et al. / Materials Science and Engineering B 114–115 (2004) 15–19 Fig. 3. Influence of the HALO implantation energy on threshold voltage for an offset between DECJ and gate edge of 2 nm, a low drain-extension doping gradient, and a HALO dose of 5.0 × 1013 cm−2 . the source-channel potential barrier. This way the electrical the depth and lower energy towards the interface. A too low channel length is increased and the threshold voltage roll-off HALO implantation energy results in a high dopant dose loss behavior is improved for a given physical gate length keeping in the poly-silicon gate and in the surrounding oxide. There- overlap capacitance and saturation current nearly unchanged. fore, there should be an optimum for the HALO implantation The main task is to form the HALO profile in such a way that energy. Fig. 3 shows the effect of the HALO implantation the net concentration at the channel side close to the DECJ is energy on the threshold voltage roll-off. One can clearly see high enough and the decrease of the channel profile towards that extremely low and extremely high energies result in bad the center of the channel is strong enough in order to avoid a roll-off characteristics, whereas the medium energies show a significant lowering of the saturation current. The extension better roll-off behavior because the concentration maximum of the space charge region at the drain side of the DECJ is in is close to oxide silicon interface and DECJ, and the gradi- the range of some few nanometers, whereas the extension of ent of the HALO profile towards the middle of the channel is the space charge region at the other side of the DECJ is up to relatively high. In Table 2 the influence of the HALO implan- 10 times higher. Therefore, a reduction of that space charge tation energy on the saturation current is presented, where Ioff region should directly result in an improvement of the roll-off is kept constant. No pronounced degradation of the saturation behavior. In the following we consider different ways to con- current is observed. struct appropriate profiles using typical process parameters. First we consider the influence of the HALO implantation 4.2. Inﬂuence of tilt angle energy. Then we simulate the effect of the tilt angle. Table 3 gives an overview of the obtained tendencies. Using relatively high HALO implantation energy, tilt an- gles in the range from 25◦ to 35◦ result in the deposition of 4.1. Inﬂuence of HALO implantation energy dopant atoms deep under the poly gate fare away from the DECJ. In those cases even the doping concentration in the The HALO implantation energy controls the location of middle of the channel is dominated by the HALO implan- the maximum of the net concentration in the channel and thus tation. Any change of the dose therefore directly causes a also the concentration at the junction close to the gate oxide change of the threshold voltage, since the doping concentra- silicon interfaces. Higher energy shifts the maximum into tion in the entire channel is changed. The overlap capacitance Table 3 Influence of typical doping and process parameters on transistor performance Vth Ion Ioff Ion /Ioff Cov Roll-off behavior Increase of drain-extension doping gradient ↑ ↓ ↓ ↑ ↓ Improved Increase of HALO implantation dose ↑ ↓ ↓ ↑ Improved Influence of HALO implantation energy O O O O O Decrease of HALO implantation angle ↓ ↑ ↑ O Degraded Decrease of offset between gate edge and DECJ ↓ ↑ ↑ ↓ ↑ Degraded (↓) decrease; (↑) increase; (O) optimum to adjust; (–) no or small influence only.
A. Erlebach et al. / Materials Science and Engineering B 114–115 (2004) 15–19 19 is only slightly influenced. In general the threshold voltage hand, it has been demonstrated that optimizing the HALO roll-off behavior is becoming worse with smaller tilt angles. profile results in a better threshold voltage roll-off behavior A decrease of the tilt angle down to 25◦ should result in de- without degrading saturation current and overlap capacitance graded roll-off curves. For very low tilt angles the transistor too much. has a high off-current and is open for zero gate voltage at gate lengths shorter than 40 nm. However, a higher HALO dose could result in both good roll-off behavior and high satura- Acknowledgement tion current. Further investigations are necessary to confirm this. This work has been partially supported by EU grant IST- 2001-32061 (IMPULSE project). 5. Conclusion References It has been shown by process and device simulation that the improvement of the roll-off behavior of a deep sub-m tran-  DIOS-ISE, ISE Integrated Systems Engineering AG, Zurich, 2004. sistor by increasing the doping gradient of the drain-extension  DESSIS-ISE, Integrated Systems Engineering AG, Zurich, 2004. profile is limited because of the collateral degradation of satu-  M.A. Darwish, J.L. Lentz, M.R. Pinto, P.M. Zeitzoff, T.J. Krutsick, ration current and overlap capacitance. The compensation of H.H. Vuong, IEEE Trans. Electron Devices 44 (1997) 1529–1538. the degradation of Ion and Cov deteriorates the roll-off behav-  J.D. Bude, MOSFET Modeling into the ballistic regime, SISPAD 2000, Seattle. ior. Hence the doping profile gradient of the drain-extension  F.M. Bufler, Y. Asahi, H. Yoshimura, C. Zechner, A. Schenk, W. profile is not the proper parameter for improving the tran- Fichtner, IEEE Trans. Electron Devices 50 (2003) 418–424. sistor performance under these circumstances. On the other  ITRS Roadmap, 2003.
You can also read
Next slide ... Cancel